1 STANDARD STEELS 403 STANDARD STEELS Standard Steels Compositions, Applications, and Heat Treatments Steel is the generic term for a large family of iron carbon alloys, which are malleable, within some temperature range, immediately after solidification from the molten state. The principal raw materials used in steelmaking are iron ore, coal, and limestone. These materials are converted in a blast furnace into a product known as pig iron, which contains considerable amounts of carbon, manganese, sulfur, phosphorus, and silicon. Pig iron is hard, brittle, and unsuitable for direct processing into wrought forms. Steelmaking is the process of refining pig iron as well as iron and steel scrap by removing undesirable elements from the melt and then adding desirable elements in predetermined amounts. A primary reaction in most steelmaking is the combination of carbon with oxygen to form a gas. If dissolved oxygen is not removed from the melt prior to or during pouring, the gaseous products continue to evolve during solidification. If the steel is strongly deoxidized by the addition of deoxidizing elements, no gas is evolved, and the steel is called killed because it lies quietly in the molds. Increasing degrees of gas evolution (decreased deoxidation) characterize steels called semikilled, capped, or rimmed. The degree of deoxidation affects some of the properties of the steel. In addition to oxygen, liquid steel contains measurable amounts of dissolved hydrogen and nitrogen. For some critical steel applications, special deoxidation practices as well as vacuum treatments may be used to reduce and control dissolved gases. The carbon content of common steel grades ranges from a few hundredths of a per cent to about 1 per cent. All steels also contain varying amounts of other elements, principally manganese, which acts as a deoxidizer and facilitates hot working. Silicon, phosphorus, and sulfur are also always present, if only in trace amounts. Other elements may be present, either as residuals that are not intentionally added, but result from the raw materials or steelmaking practice, or as alloying elements added to effect changes in the properties of the steel. Steels can be cast to shape, or the cast ingot or strand can be reheated and hot worked by rolling, forging, extrusion, or other processes into a wrought mill shape. Wrought steels are the most widely used of engineering materials, offering a multitude of forms, finishes, strengths, and usable temperature ranges. No other material offers comparable versatility for product design. Numbering Systems for Metals and Alloys. Several different numbering systems have been developed for metals and alloys by various trade associations, professional engineering societies, standards organizations, and by private industries for their own use. The numerical code used to identify the metal or alloy may or may not be related to a specification, which is a statement of the technical and commercial requirements that the product must meet. Numbering systems in use include those developed by the American Iron and Steel Institute (AISI), Society of Automotive Engineers (SAE), American Society for Testing and Materials (ASTM), American National Standards Institute (ANSI), Steel Founders Society of America, American Society of Mechanical Engineers (ASME), American Welding Society (AWS), Aluminum Association, Copper Development Association, U.S. Department of Defense (Military Specifications), and the General Accounting Office (Federal Specifications). The Unified Numbering System (UNS) was developed through a joint effort of the ASTM and the SAE to provide a means of correlating the different numbering systems for metals and alloys that have a commercial standing. This system avoids the confusion caused when more than one identification number is used to specify the same material, or when the same number is assigned to two entirely different materials. It is important to understand that a UNS number is not a specification; it is an identification number for metals and alloys for which detailed specifications are provided elsewhere. UNS numbers are shown in Table 1; each number consists of a letter prefix followed by five digits. In some, the letter is suggestive of the family of metals identified by the series, such as A for alumi-
2 404 NUMBERING SYSTEMS num and C for copper. Whenever possible, the numbers in the UNS groups contain numbering sequences taken directly from other systems to facilitate identification of the material; e.g., the corresponding UNS number for AISI 1020 steel is G The UNS numbers corresponding to the commonly used AISI-SAE numbers that are used to identify plain carbon alloy and tool steels are given in Table 1. Table 1. Unified Numbering System (UNS) for Metals and Alloys UNS Series A00001 to A99999 C00001 to C99999 D00001 to D99999 E00001 to E99999 Metal Aluminum and aluminum alloys Copper and copper alloys Specified mechanical property steels Rare earth and rare earthlike metals and alloys F00001 to F99999 G00001 to G99999 H00001 to H99999 J00001 to J99999 Cast irons AISI and SAE carbon and alloy steels (except tool steels) AISI and SAE H-steels Cast steels (except tool steels) K00001 to K99999 L00001 to L99999 M00001 to M99999 N00001 to N99999 Miscellaneous steels and ferrous alloys Low-melting metals and alloys Miscellaneous nonferrous metals and alloys Nickel and nickel alloys P00001 to P99999 R00001 to R99999 S00001 to S99999 T00001 to T99999 Precious metals and alloys Reactive and refractory metals and alloys Heat and corrosion resistant (stainless) steels Tool steels, wrought and cast W00001 to W99999 Z00001 to Z99999 Welding filler metals Zinc and zinc alloys
3 NUMBERING SYSTEMS 405 Table 1. AISI and SAE Numbers and Their Corresponding UNS Numbers for Plain Carbon, Alloy, and Tool Steels AISI-SAE Numbers UNS Numbers AISI-SAE Numbers UNS Numbers AISI-SAE Numbers UNS Numbers AISI-SAE Numbers UNS Numbers Plain Carbon Steels 1005 G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G G L14 G G G G15610 Alloy Steels 1330 G G G G G G G G G G G G G G G G G40230 E4340 G43406 E51100 G G G G46150 E52100 G G G G G G G G G B44 G G G G B46 G G G G B50 G G G G B60 G G G G B60 G G G G B45 G G G G B17 G G G G B30 G G G G G G G86400 Tool Steels (AISI and UNS Only) M1 T11301 T6 T12006 A6 T30106 P4 T51604 M2 T11302 T8 T12008 A7 T30107 P5 T51605 M4 T11304 T15 T12015 A8 T30108 P6 T51606 M6 T11306 H10 T20810 A9 T30109 P20 T51620 M7 T11307 H11 T20811 A10 T30110 P21 T51621 M10 T11310 H12 T20812 D2 T30402 F1 T60601 M3-1 T11313 H13 T20813 D3 T30403 F2 T60602 M3-2 T11323 H14 T20814 D4 T30404 L2 T61202 M30 T11330 H19 T20819 D5 T30405 L3 T61203 M33 T11333 H21 T20821 D7 T30407 L6 T61206 M34 T11334 H22 T20822 O1 T31501 W1 T72301 M36 T11336 H23 T20823 O2 T31502 W2 T72302 M41 T11341 H24 T20824 O6 T31506 W5 T72305 M42 T11342 H25 T20825 O7 T31507 CA2 T90102 M43 T11343 H26 T20826 S1 T41901 CD2 T90402 M44 T11344 H41 T20841 S2 T41902 CD5 T90405 M46 T11346 H42 T20842 S4 T41904 CH12 T90812 M47 T11347 H43 T20843 S5 T41905 CH13 T90813 T1 T12001 A2 T30102 S6 T41906 CO1 T91501 T2 T12002 A3 T30103 S7 T41907 CS5 T91905 T4 T12004 A4 T30104 P2 T51602 T5 T12005 A5 T30105 P3 T51603
4 406 NUMBERING SYSTEMS Standard Steel Classification. Wrought steels may be classified systematically into groups based on some common characteristic, such as chemical composition, deoxidation practice, finishing method, or product form. Chemical composition is the most often used basis for identifying and assigning standard designations to wrought steels. Although carbon is the principal hardening and strengthening element in steel, no single element controls the steel s characteristics. The combined effect of several elements influences response to heat treatment, hardness, strength, microstructure, corrosion resistance, and formability. The standard steels can be divided broadly into three main groups: carbon steels, alloy steels, and stainless steels. Carbon Steels: A steel qualifies as a carbon steel when its manganese content is limited to 1.65 per cent (max), silicon to 0.60 per cent (max), and copper to 0.60 per cent (max). With the exception of deoxidizers and boron when specified, no other alloying elements are added intentionally, but they may be present as residuals. If any of these incidental elements are considered detrimental for special applications, maximum acceptable limits may be specified. In contrast to most alloy steels, carbon steels are most often used without a final heat treatment; however, they may be annealed, normalized, case hardened, or quenched and tempered to enhance fabrication or mechanical properties. Carbon steels may be killed, semikilled, capped, or rimmed, and, when necessary, the method of deoxidation may be specified. Alloy Steels: Alloy steels comprise not only those grades that exceed the element content limits for carbon steel, but also any grade to which different elements than used for carbon steel are added, within specific ranges or specific minimums, to enhance mechanical properties, fabricating characteristics, or any other attribute of the steel. By this definition, alloy steels encompass all steels other than carbon steels; however, by convention, steels containing over 3.99 per cent chromium are considered special types of alloy steel, which include the stainless steels and many of the tool steels. In a technical sense, the term alloy steel is reserved for those steels that contain a modest amount of alloying elements (about 1 4 per cent) and generally depend on thermal treatments to develop specific mechanical properties. Alloy steels are always killed, but special deoxidation or melting practices, including vacuum, may be specified for special critical applications. Alloy steels generally require additional care throughout their manufacture, because they are more sensitive to thermal and mechanical operations. Stainless Steels: Stainless steels are high-alloy steels and have superior corrosion resistance to the carbon and conventional low-alloy steels because they contain relatively large amounts of chromium. Although other elements may also increase corrosion resistance, their usefulness in this respect is limited. Stainless steels generally contain at least 10 per cent chromium, with or without other elements. It has been customary in the United States, however, to include in the stainless steel classification those steels that contain as little as 4 per cent chromium. Together, these steels form a family known as the stainless and heat-resisting steels, some of which possess very high strength and oxidation resistance. Few, however, contain more than 30 per cent chromium or less than 50 per cent iron. In the broadest sense, the standard stainless steels can be divided into three groups based on their structures: austenitic, ferritic, and martensitic. In each of the three groups, there is one composition that represents the basic, general-purpose alloy. All other compositions are derived from the basic alloy, with specific variations in composition being made to obtain very specific properties. The austenitic grades are nonmagnetic in the annealed condition, although some may become slightly magnetic after cold working. They can be hardened only by cold working, and not by heat treatment, and combine outstanding corrosion and heat resistance with good mechanical properties over a wide temperature range. The austenitic grades are further classified into two subgroups: the chromium nickel types and the less frequently used
5 AISI-SAE No. NUMBERING SYSTEMS 407 Table 2. Composition of AISI-SAE Standard Carbon Steels UNS No. Composition(%) a C Mn P(max) b S(max) b Nonresulfurized Grades 1 per cent Mn (max) 1005 c G max 0.35 max c G max G max G G G G G G G G G G G G G G G G G G G G G G G G G G G G G c G G c G c G c G G G G G c G G G
6 408 NUMBERING SYSTEMS Table 2. (Continued) Composition of AISI-SAE Standard Carbon Steels AISI-SAE No. UNS No. Composition(%) a C Mn P(max) b S(max) b Nonresulfurized Grades Over 1 per cent Mn 1513 G G G G G G G G G G G Free-Machining Grades Resulfurized 1110 G G G G G G G G G G Free-Machining Grades Resulfurized and Rephosphorized 1211 G max G max G max G max L14 d G max a The following notes refer to boron, copper, lead, and silicon additions: Boron: Standard killed carbon steels, which are generally fine grain, may be produced with a boron treatment addition to improve hardenability. Such steels are produced to a range of per cent B. These steels are identified by inserting the letter B between the second and third numerals of the AISI or SAE number, e.g., 10B46. Copper: When copper is required, 0.20 per cent (min) is generally specified. Lead: Standard carbon steels can be produced with a lead range of per cent to improve machinability. Such steels are identified by inserting the letter L between the second and third numerals of the AISI or SAE number, e.g., 12L15 and 10L45. Silicon: It is not common practice to produce the 12XX series of resulfurized and rephosphorized steels to specified limits for silicon because of its adverse effect on machinability. When silicon ranges or limits are required for resulfurized or nonresulfurized steels, however, these values apply: a range of 0.08 per cent Si for Si max up to 0.15 per cent inclusive, a range of 0.10 per cent Si for Si max over 0.15 to 0.20 per cent inclusive, a range of 0.15 per cent Si for Si max over 0.20 to 0.30 per cent inclusive, and a range of 0.20 per cent Si for Si max over 0.30 to 0.60 per cent inclusive. Example: Si max is 0.25 per cent, range is per cent. b Values given are maximum percentages, except where a range of values is given. c Standard grades for wire rods and wire only. d per cent Pb.
7 NUMBERING SYSTEMS 409 chromium manganese low nickel types. The basic composition in the chromium nickel group is widely known as 18 8 (Cr Ni) and is the general-purpose austenitic grade. This grade is the basis for over 20 modifications that can be characterized as follows: the chromium nickel ratio has been modified to change the forming characteristics; the carbon content has been decreased to prevent intergranular corrosion; the elements niobium or titanium have been added to stabilize the structure; or molybdenum has been added or the chromium and nickel contents have been increased to improve corrosion or oxidation resistance. The standard ferritic grades are always magnetic and contain chromium but no nickel. They can be hardened to some extent by cold working, but not by heat treatment, and they combine corrosion and heat resistance with moderate mechanical properties and decorative appeal. The ferritic grades generally are restricted to a narrower range of corrosive conditions than the austenitic grades. The basic ferritic grade contains 17 per cent chromium. In this series, there are free-machining modifications and grades with increased chromium content to improve scaling resistance. Also in this ferritic group is a 12 per cent chromium steel (the basic composition of the martensitic group) with other elements, such as aluminum or titanium, added to prevent hardening. The standard martensitic grades are magnetic and can be hardened by quenching and tempering. They contain chromium and, with two exceptions, no nickel. The basic martensitic grade normally contains 12 per cent chromium. There are more than 10 standard compositions in the martensitic series; some are modified to improve machinability and others have small additions of nickel or other elements to improve the mechanical properties or their response to heat treatment. Still others have greatly increased carbon content, in the tool steel range, and are hardenable to the highest levels of all the stainless steels. The martensitic grades are excellent for service in mild environments such as the atmosphere, freshwater, steam, and weak acids, but are not resistant to severely corrosive solutions. Standard Steel Numbering System. The most widely used systems for identifying wrought carbon, low alloy, and stainless steels are based on chemical composition, and are those of the American Iron and Steel Institute (AISI) and the Society of Automotive Engineers (SAE). These systems are almost identical, but they are carefully coordinated. The standard steels so designated have been developed cooperatively by producers and users and have been found through long experience to cover most of the wrought ferrous metals used in automotive vehicles and related equipment. These designations, however, are not specifications, and should not be used for purchasing unless accompanied by supplementary information necessary to describe commercially the product desired. Engineering societies, associations, and institutes whose members make, specify, or purchase steel products publish standard specifications, many of which have become well known and respected. The most comprehensive and widely used specifications are those published by the American Society for Testing and Materials (ASTM). The U.S. government and various companies also publish their own specification for steel products to serve their own special procurement needs. The Unified Numbering System (UNS) for metals and alloys is also used to designate steels (see pages 403 and 405). The numerical designation system used by both AISI and SAE for wrought carbon, alloy, and stainless steels is summarized in Table 3. Table 2 lists the compositions of the standard carbon steels; Table 4 lists the standard low alloy steel compositions; and Table 5 includes the typical compositions of the standard stainless steels.
8 410 NUMBERING SYSTEMS Table 3. AISI-SAE System of Designating Carbon and Alloy Steels AISI-SAE Designation a Type of Steel and Nominal Alloy Content (%) Carbon Steels 10xx Plain Carbon (Mn 1.00% max.) 11xx Resulfurized 12xx Resulfurized and Rephosphorized 15xx Plain Carbon (Max. Mn range 1.00 to 1.65%) Manganese Steels 13xx Mn 1.75 Nickel Steels 23xx Ni xx Ni 5.00 Nickel Chromium Steels 31xx Ni 1.25; Cr 0.65 and xx Ni 1.75; Cr xx Ni 3.50; Cr 1.50 and xx Ni 3.00; Cr 0.77 Molybdenum Steels 40xx Mo 0.20 and xx Mo 0.40 and 0.52 Chromium Molybdenum Steels 41xx Cr 0.50, 0.80, and 0.95; Mo 0.12, 0.20, 0.25, and 0.30 Nickel Chromium Molybdenum Steels 43xx Ni 1.82; Cr 0.50 and 0.80; Mo BVxx Ni 1.82; Cr 0.50; Mo 0.12 and 0.35; V 0.03 min. 47xx Ni 1.05; Cr 0.45; Mo 0.20 and xx Ni 0.30; Cr 0.40; Mo xx Ni 0.55; Cr 0.50; Mo xx Ni 0.55; Cr 0.50; Mo xx Ni 0.55; Cr 0.50; Mo xx Ni 3.25; Cr 1.20; Mo xx Ni 0.45; Cr 0.40; Mo xx Ni 0.55; Cr 0.20; Mo xx Ni 1.00; Cr 0.80; Mo 0.25 Nickel Molybdenum Steels 46xx Ni 0.85 and 1.82; Mo 0.20 and xx Ni 3.50; Mo 0.25 Chromium Steels 50xx Cr 0.27, 0.40, 0.50, and xx Cr 0.80, 0.87, 0.92, 0.95, 1.00, and xxx Cr 0.50; C 1.00 min. 51xxx Cr 1.02; C 1.00 min. 52xxx Cr 1.45; C 1.00 min. Chromium Vanadium Steels 61xx Cr 0.60, 0.80, and 0.95; V 0.10 and 0.15 min Tungsten Chromium Steels 72xx W 1.75; Cr 0.75 Silicon Manganese Steels 92xx Si 1.40 and 2.00; Mn 0.65, 0.82, and 0.85; Cr 0.00 and 0.65 High Strength Low Alloy Steels 9xx Various SAE grades xxbxx B denotes boron steels xxlxx L denotes leaded steels AISI SAE Stainless Steels 2xx 302xx Chromium Manganese Nickel Steels 3xx 303xx Chromium Nickel Steels 4xx 514xx Chromium Steels 5xx 515xx Chromium Steels a xx in the last two digits of the carbon and low alloy designations (but not the stainless steels) indicates that the carbon content (in hundredths of a per cent) is to be inserted.
9 Table 4. Compositions of AISI-SAE Standard Alloy Steels AISI-SAE No. UNS No. Composition (%) a,b C Mn P (max) S (max) Si Ni Cr Mo 1330 G G G G G G G G G G G G G G G G G G G G G E4340 c G G G G G G G G G G G G G G G G G NUMBERING SYSTEMS 411
10 AISI-SAE No. UNS No. Table 4. (Continued) Compositions of AISI-SAE Standard Alloy Steels Composition (%) a,b C Mn P (max) S (max) Si Ni Cr Mo E51100 c G E52100 c G G V 6150 G V min 8615 G G G G G G G G G G G G G G G G Standard Boron Grades d 50B44 G B46 G B50 G B60 G B60 G B45 G B17 G B30 G a Small quantities of certain elements are present that are not specified or required. These incidental elements may be present to the following maximum amounts: Cu, 0.35 per cent; Ni, 0.25 per cent; Cr, 0.20 per cent; and Mo, 0.06 per cent. b Standard alloy steels can also be produced with a lead range of per cent. Such steels are identified by inserting the letter L between the second and third numerals of the AISI or SAE number, e.g., 41L40. c Electric furnace steel. d per cent B. Source:American Iron and Steel Institute: Steel Products Manual. 412 NUMBERING SYSTEMS
11 NUMBERING SYSTEMS 413 Table 5. Standard Stainless Steels Typical Compositions AISI Type (UNS) Typical Composition (%) 201 (S20100) 202 (S20200) 205 (S20500) 301 (S30100) 302 (S30200) 302B (S30215) 303 (S30300) 303Se (S30323) 304 (S30400) 304L (S30403) 304 Cu (S30430) 304N (S30451) 305 (S30500) 308 (S30800) 309 (S30900) 309S (S30908) 405 (S40500) 409 (S40900) 429 (S42900) 430 (S43000) 430F (S43020) Cr, Ni, 0.15 C, Mn, 0.75 Si, P, S, 0.25 N Cr, 4 6 Ni, 0.15 C, Mn, 0.75 Si, P, S, 0.25 N Cr, Ni, C, Mn, 0.75 Si, P, S, N Cr, 6 8 Ni, 0.15 C, 2.0 Mn, 0.75 Si, P, S Cr, 8 10 Ni, 0.15 C, 2.0 Mn, 0.75 Si, P, S, 0.10 N Cr, 8 10 Ni, 0.15 C, 2.0 Mn, Si, P, S Cr, 8 10 Ni, 0.15 C, 2.0 Mn, 1.0 Si, 0.20 P, S min, 0.60 Mo (optional) Cr, 8 10 Ni, 0.15 C, 2.0 Mn, 1.0 Si, 0.20 P, S, 0.15 Se min Cr, Ni, 0.08 C, 2.0 Mn, 0.75 Si, P, S, 0.10 N Cr, 8 12 Ni, 0.03 C, 2.0 Mn, 0.75 Si, P, S, 0.10 N Cr, 8 10 Ni, 0.08 C, 2.0 Mn, 0.75 Si, P, S, 3 4 Cu Cr, Ni, 0.08 C, 2.0 Mn, 0.75 Si, P, S, N Cr, Ni, 0.12 C, 2.0 Mn, 0.75 Si, P, S Cr, Ni, 0.08 C, 2.0 Mn, 1.0 Si, P, S Cr, Ni, 0.20 C, 2.0 Mn, 1.0 Si, P, S Cr, Ni, 0.08 C, 2.0 Mn, 1.0 Si, P, S Ferritic Cr, 0.08 C, 1.0 Mn, 1.0 Si, P, S, Al, 0.60 max Cr, 0.08 C, 1.0 Mn, 1.0 Si, P, S, 0.05 Ni (Ti 6 C, but with 0.75 max) Cr, 0.12 C, 1.0 Mn, 1.0 Si, P, 030 S, 0.75 Ni Cr, 0.12 C, 1.0 Mn, 1.0 Si, P, 030 S, 0.75 Ni Cr, 0.12 C, 1.25 Mn, 1.0 Si, P, 0.15 S min, 0.60 Mo (optional) AISI Type (UNS) Typical Composition (%) Austenitic 310 (S31000) 310S (S31008) 314 (S31400) 316 (S31600) 316L (S31603) 316F (S31620) 316N (S31651) 317 (S31700) 317L (S31703) 321 (S32100) 329 (S32900) 330 (N08330) 347 (S34700) 348 (S34800) 384 (S38400) 430FSe (S43023) 434 (S43400) 436 (S43600) 442 (S44200) 446 (S44600) Cr, Ni, 0.25 C, 2.0 Mn, 1.5 Si, P, S Cr, Ni, 0.08 C, 2.0 Mn, 1.5 Si, P, 0.30 S Cr, Ni, 0.25 C, 2.0 Mn, Si, P, S Cr, Ni, 0.08 C, 2.0 Mn, 0.75 Si, P, S, Mo, 0.10 N Cr, Ni, 0.03 C, 2.0 Mn, 0.75 Si, P, S, Mo, 0.10 N Cr, Ni, 0.08 C, 2.0 Mn, 1.0 Si, 0.20 P, 0.10 S min, Mo Cr, Ni, 0.08 C, 2.0 Mn, 0.75 Si, P, S, 2 3 Mo, N Cr, Ni, 0.08 C, 2.0 Mn, 0.75 Si, P, S, Mo, 0.10 N max Cr, Ni, 0.03 C, 2.0 Mn, 0.75 Si, P, S, 3 4 Mo, 0.10 N max Cr, 9 12 Ni, 0.08 C, 2.0 Mn, 0.75 Si, P, S [Ti, 5(C + N) min, 0.70 max], 0.10 max Cr, Ni, 0.08 C, 2.0 Mn, 0.75 Si, P, S, 1 2 Mo Cr, Ni, 0.08 C, 2.0 Mn, Si, P, S Cr, 9 13 Ni, 0.08 C, 2.0 Mn, 0.75 Si, P, S (Nb + Ta, 10 C min, 1 max) Cr, 9 13 Ni, 0.08 C, 2.0 Mn, 0.75 Si, P, S (Nb + Ta, 10 C min, 1 max, but 0.10 Ta max), 0.20 Ca Cr, Ni, 0.08 C, 2.0 Mn, 1.0 Si, P, S Cr, 0.12 C, 1.25 Mn, 1.0 Si, P, S, 0.15 Se min Cr, 0.12 C, 1.0 Mn, 1.0 Si, P, S, Mo Cr, 0.12 C, 1.0 Mn, 1.0 Si, P, S, Mo (Nb + Ta 5 C min, 0.70 max) Cr, 0.20 C, 1.0 Mn, 1.0 Si, P, S Cr, 0.20 C, 1.5 Mn, 1.0 Si, P, S, N
12 414 NUMBERING SYSTEMS 403 (S40300) 410 (S41000) 414 (S41400) 416 (S41600) 416Se (S41623) 420 (S42000) 501 (S50100) Table 5. (Continued) Standard Stainless Steels Typical Compositions AISI Type (UNS) Typical Composition (%) Cr, 1.15 C, 1.0 Mn, 0.5 Si, P, S, 0.60 Ni Cr, 0.15 C, 1.0 Mn, 1.0 Si, P, S, 0.75 Ni Cr, Ni, 0.15 C, 1.0 Mn, 1.0 Si, P, S, Ni Cr, 0.15 C, 1.25 Mn, 1.0 Si, P, 0.15 S min, Mo (optional) Cr, 0.15 C, 1.25 Mn, 1.0 Si, P, S, 0.15 Se min Cr, 0.15 C min, 1.0 Mn, 1.0 Si, P, S 4 6 Cr, 0.10 C min, 1.0 Mn, 1.0 Si, P, S, Mo AISI Type (UNS) Typical Composition (%) Martensitic Heat-Resisting 420F (S42020) 422 (S42200) 431 (S41623) 440A (S44002) 440B (S44003) 440C (S44004) 502 (S50200) Cr, over 0.15 C, 1.25 Mn, 1.0 Si, P, 0.15 S min, 0.60 Mo max (optional) Cr, Ni, C, Mn, 0.50 Si, P, S, Mo, V, W Cr, Ni, 0.20 C, 1.0 Mn, 1.0 Si, P, S Cr, C, 1.0 Mn, 1.0 Si, P, S, 0.75 Mo Cr, C, 1.0 Mn, 1.0 Si, P, S, 0.75 Mo Cr, C, 1.0 Mn, 1.0 Si, 0040 P, S, 0.75 Mo 4 6 Cr, 0.10 C. 1.0 Mn, 1.0 Si, P, S, Mo Thermal Treatment of Steel. Steel s versatility is due to its response to thermal treatment. Although most steel products are used in the as-rolled or un-heat-treated condition, thermal treatment greatly increases the number of properties that can be obtained, because at certain critical temperatures iron changes from one type of crystal structure to another. This structural change, known as an allotropic transformation, is spontaneous and reversible and can be made to occur by simply changing the temperature of the metal. In steel, the transformation in crystal structure occurs over a range of temperatures, bounded by lower and upper critical points. When heated, most carbon and low alloy steels have a critical temperature range between 1300 and 1600 degrees F. Steel above this temperature, but below the melting range, has a crystalline structure known as austenite, in which the carbon and alloying elements are dissolved in a solid solution. Below this critical range, the crystal structure changes to a phase known as ferrite, which is capable of maintaining only a very small percentage of carbon in solid solution. The remaining carbon exists in the form of carbides, which are compounds of carbon and iron and certain of the other alloying elements. Depending primarily on cooling rate, the carbides may be present as thin plates alternating with the ferrite (pearlite); as spheroidal globular particles at ferrite grain boundaries or dispersed throughout the ferrite; or as a uniform distribution of extremely fine particles throughout a ferritelike phase, which has an acicular (needlelike) appearance, named martensite. In some of the highly alloyed stainless steels the addtion of certain elements stabilizes the austenite structure so that it persists even at very low temperatures (austenitic grades). Other alloying elements can prevent the formation of austenite entirely up to the melting point (ferritic grades). Fundamentally, all steel heat treatments are intended to either harden or soften the metal. They involve one or a series of operations in which the solid metal is heated and cooled under specified conditions to develop a required structure and properties. In general, there are five major forms of heat treatment for the standard steels that modify properties to suit either fabrication or end use. Quenching and Tempering: The primary hardening treatment for steel, quenching and tempering, usually consists of three successive operations: heating the steel above the critical range and holding it at these temperatures for a sufficient time to approach a uniform solid solution (austenitizing); cooling the steel rapidly by quenching in oil, water, brine,
13 NUMBERING SYSTEMS 415 salt or air to form a hard, usually brittle, metastable structure known as untempered or white martensite; tempering the steel by reheating it to a temperature below the critical range in order to obtain the required combination of hardness, strength, ductility, toughness, and structural stability (tempered martensite). Two well-known modifications of conventional quenching and tempering are austempering and martempering. They involve interrupted quenching techniques (two or more quenching media) that can be utilized for some steels to obtain desired structures and properties while minimizing distortion and cracking problems that may occur in conventional hardening. Normalizing: The steel is heated to a temperature above the critical range, after which it is cooled in still air to produce a generally fine pearlite structure. The purpose is to promote uniformity of structure and properties after a hot-working operation such as forging or extrusion. Steels may be placed in service in the normalized condition, or they may be subjected to additional thermal treatment after subsequent machining or other operations. Annealing: The steel is heated to a temperature above or within the critical range, then cooled at a predetermined slow rate (usually in a furnace) to produce a coarse pearlite structure. This treatment is used to soften the steel for improved machinability; to improve or restore ductility for subsequent forming operations; or to eliminate the residual stresses and microstructural effects of cold working. Spheroidize Annealing: This is a special form of annealing that requires prolonged heating at an appropriate temperature followed by slow cooling in order to produce globular carbides, a structure desirable for machining, cold forming, or cold drawing, or for the effect it will have on subsequent heat treatment. Stress Relieving: This process reduces internal stresses, caused by machining, cold working, or welding, by heating the steel to a temperature below the critical range and holding it there long enough to equalize the temperature throughout the piece. See the sections HARDENING, TEMPERING, AND ANNEALING on page 479 and HEAT-TREATING HIGH-SPEED STEELS on page 508 for more information about the heat treatment of steels. Hardness and Hardenability. Hardenability is the property of steel that determines the depth and distribution of hardness induced by quenching from the austenitizing temperature. Hardenability should not be confused with hardness as such or with maximum hardness. Hardness is a measure of the ability of a metal to resist penetration as determined by any one of a number of standard tests (Brinell, Rockwell, Vickers, etc). The maximum attainable hardness of any steel depends solely on carbon content and is not significantly affected by alloy content. Maximum hardness is realized only when the cooling rate in quenching is rapid enough to ensure full transformation to martensite. The as-quenched surface hardness of a steel part is dependent on carbon content and cooling rate, but the depth to which a certain hardness level is maintained with given quenching conditions is a function of its hardenability. Hardenability is largely determined by the percentage of alloying elements in the steel; however, austenite grain size, time and temperature during austenitizing, and prior microstructure also significantly affect the hardness depth. The hardenability required for a particular part depends on size, design, and service stresses. For highly stressed parts, the best combination of strength and toughness is obtained by through hardening to a martensitic structure followed by adequate tempering. There are applications, however, where through hardening is not necessary or even desirable. For parts that are stressed principally at or near the surface, or in which wear resistance or resistance to shock loading is anticipated, a shallow hardening steel with a moderately soft core may be appropriate. For through hardening of thin sections, carbon steels may be adequate; but as section size increases, alloy steels of increasing hardenability are required. The usual practice is to select the most economical grade that can meet the desired properties consistently. It is not
14 416 NUMBERING SYSTEMS good practice to utilize a higher alloy grade than necessary, because excessive use of alloying elements adds little to the properties and can sometimes induce susceptibility to quenching cracks. Quenching Media: The choice of quenching media is often a critical factor in the selection of steel of the proper hardenability for a particular application. Quenching severity can be varied by selection of quenching medium, agitation control, and additives that improve the cooling capability of the quenchant. Increasing the quenching severity permits the use of less expensive steels of lower hardenability; however, consideration must also be given to the amount of distortion that can be tolerated and the susceptibility to quench cracking. In general, the more severe the quenchant and the less symmetrical the part being quenched, the greater are the size and shape changes that result from quenching and the greater is the risk of quench cracking. Consequently, although water quenching is less costly than oil quenching, and water quenching steels are less expensive than those requiring oil quenching, it is important to know that the parts being hardened can withstand the resulting distortion and the possibility of cracking. Oil, salt, and synthetic water-polymer quenchants are also used, but they often require steels of higher alloy content and hardenability. A general rule for the selection of steel and quenchant for a particular part is that the steel should have a hardenability not exceeding that required by the severity of the quenchant selected. The carbon content of the steel should also not exceed that required to meet specified hardness and strength, because quench cracking susceptibility increases with carbon content. The choice of quenching media is important in hardening, but another factor is agitation of the quenching bath. The more rapidly the bath is agitated, the more rapidly heat is removed from the steel and the more effective is the quench. Hardenability Test Methods: The most commonly used method for determining hardenability is the end-quench test developed by Jominy and Boegehold, and described in detail in both SAE J406 and ASTM A255. In this test a normalized 1-inch-round, approximately 4-inch-long specimen of the steel to be evaluated is heated uniformly to its austenitizing temperature. The specimen is then removed from the furnace, placed in a jig, and immediately end quenched by a jet of room-temperature water. The water is played on the end face of the specimen, without touching the sides, until the entire specimen has cooled. Longitudinal flat surfaces are ground on opposite sides of the piece and Rockwell C scale hardness readings are taken at inch intervals from the quenched end. The resulting data are plotted on graph paper with the hardness values as ordinates (y-axis) and distances from the quenched end as abscissas (x-axis). Representative data have been accumulated for a variety of standard steel grades and are published by SAE and AISI as H-bands. These data show graphically and in tabular form the high and low limits applicable to each grade. The suffix H following the standard AISI/SAE numerical designation indicates that the steel has been produced to specific hardenability limits. Experiments have confirmed that the cooling rate at a given point along the Jominy bar corresponds closely to the cooling rate at various locations in round bars of various sizes. In general, when end-quench curves for different steels coincide approximately, similar treatments will produce similar properties in sections of the same size. On occasion it is necessary to predict the end-quench hardenability of a steel not available for testing, and reasonably accurate means of calculating hardness for any Jominy location on a section of steel of known analysis and grain size have been developed. Tempering: As-quenched steels are in a highly stressed condition and are seldom used without tempering. Tempering imparts plasticity or toughness to the steel, and is inevitably accompanied by a loss in hardness and strength. The loss in strength, however, is only incidental to the very important increase in toughness, which is due to the relief of residual stresses induced during quenching and to precipitation, coalescence, and spheroidization of iron and alloy carbides resulting in a microstructure of greater plasticity.
15 NUMBERING SYSTEMS 417 Alloying slows the tempering rate, so that alloy steel requires a higher tempering temperature to obtain a given hardness than carbon steel of the same carbon content. The higher tempering temperature for a given hardness permits a greater relaxation of residual stress and thereby improves the steel s mechanical properties. Tempering is done in furnaces or in oil or salt baths at temperatures varying from 300 to 1200 degrees F. With most grades of alloy steel, the range between 500 and 700 degrees F is avoided because of a phenomenon known as blue brittleness, which reduces impact properties. Tempering the martensitic stainless steels in the range of degrees F is not recommended because of the low and erratic impact properties and reduced corrosion resistance that result. Maximum toughness is achieved at higher temperatures. It is important to temper parts as soon as possible after quenching, because any delay greatly increases the risk of cracking resulting from the high-stress condition in the as-quenched part. Surface Hardening Treatment (Case Hardening). Many applications require high hardness or strength primarily at the surface, and complex service stresses frequently require not only a hard, wear resistant surface, but also core strength and toughness to withstand impact stress. To achieve these different properties, two general processes are used: 1) The chemical composition of the surface is altered, prior to or after quenching and tempering; the processes used include carburizing, nitriding, cyaniding, and carbonitriding; and 2) Only the surface layer is hardened by the heating and quenching process; the most common processes used for surface hardening are flame hardening and induction hardening. Carburizing: Carbon is diffused into the part s surface to a controlled depth by heating the part in a carbonaceous medium. The resulting depth of carburization, commonly referred to as case depth, depends on the carbon potential of the medium used and the time and temperature of the carburizing treatment. The steels most suitable for carburizing to enhance toughness are those with sufficiently low carbon contents, usually below 0.03 per cent. Carburizing temperatures range from 1550 to 1750 degrees F, with the temperature and time at temperature adjusted to obtain various case depths. Steel selection, hardenability, and type of quench are determined by section size, desired core hardness, and service requirements. Three types of carburizing are most often used: 1) Liquid carburizing involves heating the steel in molten barium cyanide or sodium cyanide. The case absorbs some nitrogen in addition to carbon, thus enhancing surface hardness; 2) Gas carburizing involves heating the steel in a gas of controlled carbon content. When used, the carbon level in the case can be closely controlled; and 3) Pack carburizing, which involves sealing both the steel and solid carbonaceous material in a gas-tight container, then heating this combination. With any of these methods, the part may be either quenched after the carburizing cycle without reheating or air cooled followed by reheating to the austenitizing temperature prior to quenching. The case depth may be varied to suit the conditions of loading in service. However, service characteristics frequently require that only selective areas of a part have to be case hardened. Covering the areas not to be cased, with copper plating or a layer of commercial paste, allows the carbon to penetrate only the exposed areas. Another method involves carburizing the entire part, then removing the case in selected areas by machining, prior to quench hardening. Nitriding: The steel part is heated to a temperature of degrees F in an atmosphere of ammonia gas and dissociated ammonia for an extended period of time that depends on the case depth desired. A thin, very hard case results from the formation of nitrides. Strong nitride-forming elements (chromium and molybdenum) are required to be present in the steel, and often special nonstandard grades containing aluminum (a strong nitride former) are used. The major advantage of this process is that parts can be quenched and tempered, then machined, prior to nitriding, because only a little distortion occurs during nitriding.